Structure, properties and corrosion resistivity of polymeric nanocomposite coatings based on layered silicates.Abstract This paper reviews the recent research and development of polymeric nanocomposite coatings based on layered silicates. In the past few decades, extensive research activities have been conducted on clay minerals Clay minerals are hydrous aluminium phyllosilicates, sometimes with variable amounts of iron, magnesium, alkali metals, alkaline earths and other cations. Clays have structures similar to the micas and therefore form flat hexagonal sheets. due to their unique layered structure, rich intercalation intercalation
the insertion of certain organic compounds such as aridines and ethidium bromide that possess a planar aromatic ring structure of appropriate size and geometry so as to insert between base pairs in double-stranded DNA. chemistry and availability at low cost, environmental stability, and good processability. One of the most important categories of layered silicates is nanoclays. The nanoclay is considered as reinforcement for polymers in the manufacture of low-cost, lightweight and high performance nanocomposite coatings. In this paper, we try to introduce the structure, properties, and surface modification of clay minerals. Different properties of polymer clay Polymer clay is a sculptable material based on the polymer polyvinyl chloride. It usually contains no clay minerals, and is only called "clay" because it can be used for similar purposes as natural clay. nonocomposite coatings may consist of conductive and nonconductive polymers. The corrosion resistance of each type is discussed separately. Some novel properties can be observed from the interaction of two dissimilar chemical components at the molecular level that posses enhancements in corrosion inhibition on metallic substrates. Finally, the prospective problems of industrial usage of these materials are mentioned.
Keywords Clay minerals, Montmorrilonite, Polyaniline, Conductive polymers
Abbreviations CRS Cold-rolled Steel CEC Cation Exchange Capacity EPA Environmental Pollution Agency ICPs Intrinsically Conductive Polymers MMT Montmorillonite PANi Polyaniline PPO Polyphenylene Oxide PPS Polyphenylene Sulfide PPy Polypyrrole PS Polystyrene PSF Polysulfone PCNs Polymer Clay Nanocomposites PLS Polymer Layered Silicates PSAN Poly(styrene-co-acrylonitrile) SPI Soluble Polyimide UV Ultra Violet
Chromium-containing compounds have formed effective anticorrosive undercoatings for years, yet due to environmental and health concerns, they need to be replaced.(1-6) However, strict EPA EPA eicosapentaenoic acid.
n.pr See acid, eicosapentaenoic.
n. environmental regulations require the elimination of the heavily used chromate chromate /chro·mate/ (kro´mat) any salt of chromic acid.
A salt of chromic acid.
any salt of chromic acid. inhibitors by the year 2007. (7) Therefore, some environmentally friendly Environmentally friendly, also referred to as nature friendly, is a term used to refer to goods and services considered to inflict minimal harm on the environment. and effective corrosion-inhibitive coatings need to be urgently considered for the shipping, aerospace, and automobile industries.
As a primary method for corrosion protection of metals, coatings make a barrier by preventing the diffusion of oxygen and water. However, there is no perfect barrier coating, and all coatings eventually fail due to existing pinhole defects. Other methods, therefore, have been developed. such as chemical inhibitors, cathodic protection Cathodic protection (CP) is a technique to control the corrosion of a metal surface by making that surface the cathode of an electrochemical cell.
It is a method used to protect metal structures from corrosion. , and anodic an·ode
1. A positively charged electrode, as of an electrolytic cell, storage battery, or electron tube.
2. The negatively charged terminal of a primary cell or of a storage battery that is supplying current. protection. (8) Moreover, a protective monolayer mon·o·lay·er
1. A film or layer one molecule thick formed at the interface between water and either oil or air by a substance such as a partially esterified fatty acid that contains both hydrophobic and hydrophilic groups in the same film can be formed on the metal surface that interferes with the cathodic or anodic reaction of the corrosion cell. (9)
Nanoscale materials have unique physical, chemical, and physicochemical physicochemical /phys·i·co·chem·i·cal/ (fiz?i-ko-kem´ik-il) pertaining to both physics and chemistry.
1. Relating to both physical and chemical properties. properties, which may improve thecorrosion protection in comparison to bulk-size materials. It is well known that such nanoparticles create high specific surface area. This specification allows the uniform dispersion of nanoparticles into matrix materials with a low dosage so that the efficiency of nanocomposites can be significantly high in terms of material properties. (10)
Recently, organic-inorganic nanocomposites have attracted attention. Their remarkable properties and unique structure have led to the synthesis and study of a variety of hybrid composite materials. (11) The intercalation of inorganic materials by organic guest species is a way to construct an ordered organic-inorganic assembly. (12) Polymer intercalated in·ter·ca·lat·ed
Inserted between two others; interposed.
in·terca·late nanocomposites, prepared by using layered materials, have a high degree of polymer ordering and exhibit advanced gas barrier, thermal stability, and enhanced mechanical properties compared with pristine polymers. (13), (14) Nanocomposites differ from traditional composites due to the complex interaction of the nanostructural heterogeneous phases. In addition, the properties of nanoscopic particles differ greatly from a macroscopic macroscopic /mac·ro·scop·ic/ (mak?ro-skop´ik) gross (2).
mac·ro·scop·ic or mac·ro·scop·i·cal
1. Large enough to be perceived or examined by the unaided eye.
2. sample of the same materials. The combination of organic and inorganic materials may offer novel properties due to the synergistic effect Synergistic effect
A violation of value-additivity in that the value of a combination is greater than the sum of the individual values. of the two components.(15), (16) Since the commencement of the nanotechnology era, nanocomposites composed of polymers and inorganic particles have aroused much interest in the scientific community. To improve properties possessed by polymers and to generate new properties, researchers are formulating organic-inorganic hybrid materials using different polymers. (9)
Study of polymer clay nanocomposites is a functional field for many applications--not just exclusively directed towards improvement of mechanical properties of plastic materials--but also offers materials with other functions such as conductivity, membranes, corrosion protection, and fire retardant fire retardant Public health A chemical used to resist combustion, which may contain polybrominated biphenyls and antimony oxide behavior.(17), (18) One of the most interesting features of polymer clay nanocomposites (PCNs) is the available variety of processing options. The variety is raised from characteristics of the polymer and mechanisms of interaction with the clay. (19)
A lot of research has been done on the integration of inorganic nanolayers like montmorillonite Montmorillonite is a very soft phyllosilicate mineral that typically forms in microscopic crystals, forming a clay. It is named after Montmorillon in France. Montmorillonite, a member of the smectite family, is a 2:1 clay, meaning that it has 2 tetrahedral sheets sandwiching a (MMT MMT Million Metric Tons
MMT Médecins Maîtres-Toile
MMT Methadone Maintenance Treatment
MMT Multiple Mirror Telescope
MMT Mission Management Team (International Space Station)
MMT Military Training Technology ) clay into the organic polymeric matrices. The findings show that these materials, as a coatings layer, enhance the corrosion protection effect of steel and aluminum in comparison to pristine polymers. The primary effect of a polymeric coating is to act as a physical barrier against aggressive species such as [O.sub.2] and [H.sup.+] These inorganic materials with a plate-like shape are usually employed to effectively increase the length of the diffusion pathways for oxygen and water and decrease the permeability of the coating and lead to corrosion receptivity of coatings. (20-24)
Layered silicates, structure, and modeling
Layered silicate silicate, chemical compound containing silicon, oxygen, and one or more metals, e.g., aluminum, barium, beryllium, calcium, iron, magnesium, manganese, potassium, sodium, or zirconium. Silicates may be considered chemically as salts of the various silicic acids. clays are an interesting class of filler materials. These minerals include both natural clays(e.g., MMT, hectorite, and saponite sap·o·nite
A clay mineral that is a hydrous silicate of aluminum and magnesium and occurs in soft amorphous masses in the cavities of certain rocks.
[Latin s ) and synthesized clays (e.g., fluorohectorite, laponite, and magadiite) while MMT and hectorite are the most widely used. (25)
There are different articles in the literature on organoclays, clay-polymer interactions, or the processing aspects of clay-polymer nanocomposites. (17), (25-35) The layered structure of clay minerals used for polymer nanocomposites can be classified into three main groups that include: (a) 2:1 type, (b) 1:1 type, and (c) layered silicic acids. (25)
The clays belonging to the smectite Smec´tite
n. 1. (Min.) A hydrous silicate of alumina, of a greenish color, which, in certain states of humidity, appears transparent and almost gelatinous. family have a crystal structure consisting of nanometer thick layers (platelets) of aluminum octahedron octahedron: see polyhedron. sheet sandwiched in between two silicon tetrahedron tetrahedron: see polyhedron. sheets. Stacking of the layers leads to a van der Waals gap between the layers. Isomorphic (mathematics) isomorphic - Two mathematical objects are isomorphic if they have the same structure, i.e. if there is an isomorphism between them. For every component of one there is a corresponding component of the other. substitution of Al with Mg, Fe, and Li in the octahedron sheets, and/or Si with Al in tetrahedron sheets, gives each three-sheet layer an overall negative charge. This charge is counterbalanced by exchangeable metal cations residing in the interlayer Noun 1. interlayer - a layer placed between other layers
layer, bed - single thickness of usually some homogeneous substance; "slices of hard-boiled egg on a bed of spinach" space, such as Na, Ca, Mg, Fe, and Li.
Clays consists of layers made up of one aluminum octahedron sheet and one silicon tetrahedron sheet. Each layer bares no charge due to the absence of isomorphic substitution in either the octahedron or tetrahedron sheet. Thus, except for water molecules, neither cations nor anions occupy the space between the layers, and the layers are held together by hydrogen bonding hydrogen bonding
Interaction involving a hydrogen atom located between a pair of other atoms having a high affinity for electrons; such a bond is weaker than an ionic bond or covalent bond but stronger than van der Waals forces. between hydroxyl groups in the octahedral oc·ta·he·dral
Having eight plane surfaces.
octa·hedral·ly adv. sheets, and oxygen in the tetrahedral tet·ra·he·dral
1. Of or relating to a tetrahedron.
2. Having four faces.
tet sheets of the adjacent layers.
Layered silicic acids
Clays consist mainly of silicon tetrahedron sheets with different layer thicknesses. The basic structure is composed of layered silicate networks and interlayer hydrated hy·drat·ed
Chemically combined with water, especially existing in the form of a hydrate.
Adj. 1. hydrated - containing combined water (especially water of crystallization as in a hydrate)
hydrous alkali metal alkali metal
Any of the six chemical elements in the leftmost group of the periodic table (lithium, sodium, potassium, rubidium, cesium, and francium). They form alkalies when they combine with other elements. cations. (25).
Among the many layered materials, clay minerals (e.g., MMT) have been extensively investigated because they are natural, abundant, and inexpensive.(36) MMT--also known as 2:1 phyllosilicates--is usually used as a sorbent sorbent /sor·bent/ (sor´bent) an agent that sorbs; see absorbent and adsorbent.
an agent that sorbs. of organic compounds mainly because of the large surface area (760 X 10 e3 m[sup.2]/kg), the high cation exchange capacity In soil science, cation exchange capacity (CEC) is the capacity of a soil for ion exchange of positively charged ions between the soil and the soil solution. A positively-charged ion, which has fewer electrons than protons, is known as a cation due to its attraction to cathodes. (CEC (Central Electronic Complex) The set of hardware that defines a mainframe, which includes the CPU(s), memory, channels, controllers and power supplies included in the box. Some CECs, such as IBM's Multiprise 2000 and 3000, include data storage devices as well. ) (~1 mol k[g.sup.-1] molar monovalent monovalent /mono·va·lent/ (-va´lent)
1. having a valency of one.
2. capable of combining with only one antigenic specificity or with only one antibody specificity. cations), and relative ease of forming interlayer complexes with a wide variety of organic molecules.(37-40) Due to the above advantages, MMT is a favorable candidate for reinforcing organic polymer materials. (41) As shown in Fig. 1, the layers of clay align themselves in a parallel manner, form stacks, and areattracted to each other by a weak van der Waals force van der Waals force
A weak attractive force between atoms or nonpolar molecules caused by an instantaneous dipole moment of one atom or molecule that induces a similar temporary dipole moment in adjacent atoms or molecules. . The gap between the layers is called the gallery and the distance is called [d.sub.001] spacing, which can vary over a wide range depending on the size of the cations adsorbed.
[FIGURE 1 OMITTED]
The nature of pristine clay is hydrophilic hydrophilic /hy·dro·phil·ic/ (-fil´ik) readily absorbing moisture; hygroscopic; having strongly polar groups that readily interact with water.
adj. and the increase in interlayer spacing that occurs with swelling of the Na+-MMT clay in water causes the particles to be penetrated by relatively large molecules. (42) The normally hydrophilic silicate surface must be converted into an organophilic one to render layered silicates miscible miscible /mis·ci·ble/ (mis´i-b'l) able to be mixed.
Capable of being and remaining mixed in all proportions. Used of liquids. with other polymer matrices and make the intercalation of many engineering polymers possible. Generally, this can be done by ion-exchange interactions with cationic cationic
having qualities dependent on having free cations available.
are wetting agents that disrupt or damage cell membranes, denature proteins and inactivate enzymes. onium surfactants, including primary, secondary, tertiary, and quaternary quaternary /qua·ter·nary/ (kwah´ter-nar?e)
1. fourth in order.
2. containing four elements or groups.
1. Consisting of four; in fours. alky1 ammonium or alkylphosphonium cations. (43), (44). These organic clays are more compatible with polymers and swell in a polar solvent and easily exfoliate ex·fo·li·ate
v. ex·fo·li·at·ed, ex·fo·li·at·ing, ex·fo·li·ates
1. To remove (a layer of bark or skin, for example) in flakes or scales; peel.
2. and disperse in polymers. (45)
Two particular characteristics of layered silicates are generally considered for nanocomposites. The first is the ability of the silicate particles to disperse into individual layers. The second characteristic is the ability to fine-tune their surface chemistry through ion exchange ion exchange
A reversible chemical reaction occurring between an insoluble solid and a solution during which ions may be interchanged, used in the separation of radioactive isotopes. reactions with organic and inorganic cations. These two characteristics are, of course, interrelated in·ter·re·late
tr. & intr.v. in·ter·re·lat·ed, in·ter·re·lat·ing, in·ter·re·lates
To place in or come into mutual relationship.
in , because the degree of dispersion of nanolayered silicate in a particular polymer matrix depends on the interlayer cation cation (kăt'ī`ən), atom or group of atoms carrying a positive charge. The charge results because there are more protons than electrons in the cation. . (34)
Most of the literature about the structure and modeling of layered silicates in the nanocompositeshas focused on the type of the intercalant and the compatibility of the clay with different polymers. The processing of the clay with different functional groups, however, has attracted the most attention.
Interaction between layered silicate and polymers
The interaction among the organic and inorganic components is important because it controls the ultimate properties of the nanocomposite materials. (9) A main group of nanocomposite materials is constituted by those in which the organic polymer is confined in the inorganic layers. The inorganic layered materials exist in great variety with ordered intra-lamellar space that is potentially accessible by foreign species. They can act as matrices or hosts for polymers, yielding interesting lamellar lamellar /la·mel·lar/ (lah-mel´ar)
1. pertaining to or resembling lamellae.
2. lamellated (1).
pertaining to or emanating from lamella. organic-in-inorganic nanocomposite materials. (46)
The physical mixing of a polymer and layered silicate may not form a nanocomposite. This situation is comparable to polymer blends, where in most cases phase separation occurs. One of the differences between the nanocomposites and traditional composite is that no polymer chain penetrates into the gallery of the layered silicate, and the polymer and layers are immiscible immiscible /im·mis·ci·ble/ (i-mis´i-b'l) not susceptible to being mixed.
Incapable of being mixed or blended, as oil and water. . (13), (17), (30) In immiscible systems that typically correspond to the more conventionally filled polymers, the poor physical interaction between the organic and the inorganic components leads to poor mechanical and thermal properties. In contrast, strong interactions between the polymer and the layered silicate in nanocomposites lead to the organic and inorganic phase dispersion at the nanometer level. As a result, nanocomposites exhibit unique properties not shared by their micro counterparts or conventionally filled polymers. (28), (47-50)
The low-weight percentage of properly dispersed layered silicates throughout the polymer matrix can create a much higher surface area for polymer/filler interaction in comparison to the conventional composites. Depending on the strength of interfacial interactions between polymer matrices and layered silicates (modified or not), the following three different types of polymer layered silicate nanocomposites are thermo-dynamically achievable (see Fig. 2).
[FIGURE 2 OMITTED]
(a) Intercalated nanocomposite: The insertion of a polymer matrix into the layered silicate structure occurs in a crystallographically crys·tal·log·ra·phy
The science of crystal structure and phenomena.
crystal·log regular fashion, regardless of the clay-to-polymer ratio. Intercalated nano-composites are normally interlayered by a few molecular layers of polymer. Properties of these nanocomposites typically resemble those of ceramic materials.
(b) Flocculated nanocomposites: Conceptually, these are similar to intercalated nanocomposites. However, silicate layers are sometimes flocculated due to hydroxylated edge-edge interaction of the silicate layers.
(c) Exfoliated nanocomposite: Individual clay layers are separated in a continuous polymer matrix by an average distance that depends on the clay loading. Usually, the clay content of an exfoliated nanocomposite is much lower than that of an intercalated nanocomposite. (51) It has been claimed that a completely exfoliated morphology is required to achieve the highest properties, such as mechanical and conductivity. (46), (52)
Enhancement of material properties has been linked to the interfacial interaction between the polymer matrix and the organically modified layered silicate structure. (46) The factors that control the interaction between a particular organoclay and polymer include the cation exchange capacity (CEC) of the clay, the polarity of the reaction medium, and the chemical nature of the interlayer cations (e.g., onium ions). Proper selection of the modified clay is essential to ensure effective penetration of the polymer/monomer into the interlayer spacing of the clay, which results in the desired exfoliated or intercalated product. Further development of the compatibilizer chemistry is undoubtedly the key to the expansion of this nanocomposite technology. (53)
It is well-known that nanocomposites usually exhibit superior physical properties such as solvent resistance, ionic conductivity, (19) optical properties, (54) heat resistance, (55) decreased gas permeability, (56) and flammability, (57) better process ability, (58) thermal stability and UV susceptibility compared with various commercial polymers, (50), (59), (60) or conventional polymer composites. They also show better mechanical properties such as tensile modulus and strength which may be due to the synergy caused by host-guest interactions. (17)
Most of the works in this field focus on the morphology of the nanocomposites and different processing of the polymer and the layered silicates (i.e., in situ In place. When something is "in situ," it is in its original location. polymerization polymerization
Any process in which monomers combine chemically to produce a polymer. The monomer molecules—which in the polymer usually number from at least 100 to many thousands—may or may not all be the same. , melt interaction, and solution interaction). The other interesting subjects in this field are the characterization techniques and evaluation of properties.
Corrosion resistivity resistivity
Electrical resistance of a conductor of unit cross-sectional area and unit length. The resistivity of a conductor depends on its composition and its temperature. of nanocomposite coatings based on conductive polymers and layered silicates
There are many references about the corrosion resistance of electroactive polymers Electroactive Polymers or EAPs are polymers whose shape is modified when a voltage is applied to them. They can be used as actuators or sensors. As actuators, they are characterized by the fact that they can undergo a large amount of deformation while sustaining large forces. such as polyaniline (PANi) (61-72) poly-n-ethylaniline, (73) polyphenylene oxide, (74) and poly (2,5-bis (N-methy1-N-hexylamine) -p-phenylene vinylene (75) as pigment in paint or coatings. Because the mechanisms of corrosion protection in conductive polymers are complex and affected by many factors, several mechanisms have been proposed to explain the nature of protection with these materials. Some researchers believe that the ICP (1) (Internet Cache Protocol) A protocol used by one proxy server to query another for a cached Web page without having to go to the Internet to retrieve it. See CARP and proxy server. coatings protect aluminum and steel simply by creating a barrier mechanism, but others say that ICP coatings aid in the formation of a passive oxide film on the metal surface through an oxidation-reduction process. (67), (68) Another mechanism for corrosion protection is suggested to be anodic (i.e., the polyaniline film withdraws change from the metal and passivates its surfaces against corrosion). (76) Based on this mechanism, the role of polyaniline in active corrosion protection is due to its ability to intercept electrons on the metal surface and to transport them to the outside of the coating. (77) It is believed that the presence of layered silicates improves the corrosion resistance of the ICP coatings, not only with decreasing the coating porosity and decreasing permeability of gases and liquids, but also with stabilizing their electronic structure. (9) Recently, researchers have found that incorporation of theinorganic nanolayers of MMT clay into the polymeric matrix effectively enhance the corrosion protection of pristine conducting polymers (e.g., PANi (20), (78) poly (0-methoxyaniline), (79) poly (0-ethoxyaniline), (21) poly (3-alkylthiophene), (80) polypyrrole, (81) and pani-thiokol rubber. (82) These findings have resulted from a series of electrochemical electrochemical /elec·tro·chem·i·cal/ (-kem´i-k'l) pertaining to interaction or interconversion of chemical and electrical energies.
adj. corrosion measurements in different corrosive environments.
Among the conducting polymers, incorporation of layered silicates into the PANi and polypyrrole (PPy) has been of particular interest. These two polymers have a wide application and they have been evaluated as anticorrosive coatings for about two decades. (83-89)
Chang and coworkers (90) presented the first evaluation of the corrosion protection effects of a series of PANi/Na+-MMT clay nanocomposites by in situ emulsion polymerization Emulsion polymerization is a type of radical polymerization that usually starts with an emulsion incorporating water, monomer, and surfactant. The most common type of emulsion polymerization is an oil-in-water emulsion, in which droplets of monomer (the oil) are emulsified (with through standard electrochemical corrosion measurements. They reported significant improvement in corrosion resistance of the PANi coating on cold rolled steel (CRS CRS Course
CRS Certified Residential Specialist (real estate certification)
CRS Central Reservation System
CRS Can't Remember Stuff (polite form)
CRS Cost Reduction Strategy
CRS Consumer Relations Specialist ) with the incorporation of clay.
As shown in the schematic view of the nanocomposite coating based on PANi and clay (see Fig. 3), the presence of clay in nanoscale dispersion lengthens the diffusion path of corrosive media and improves the barrier properties. (9)
[FIGURE 3 OMITTED]
As shown in Fig. 3, clay also has a possible positive effect on protecting PANi from UV damage. In addition, clay platelets will improve the thermal stability of the ICPs. Consequently, the service life of the conducting polymer coatings can be significantly improved by the incorporation of clay.
In spite of the numerous studies about the corrosion resistance properties of PCN 1. PCN - Program Composition Notation.
2. (communications) PCN - Personal Communication Network. coatings based on ICP and layered silicates, the unsolved problem is the issue of electrical conductivity. Electrical conductivity of ICPs has always been of great interest to scientists; however, the effect of clay incorporation (a dielectric material) on the conductivity of the compound is unclear. Although the clay layers can be regarded as insulators, (25) these minerals in the conductive polymer matrix exhibit unique electrical properties due to their ionic conductivity. It is an interesting phenomenon inthe PCN coatings that the incorporation of clay did not decrease the conductivity of ICP--on the contrary, the conductivity is enhanced. (9), (29), (91) It is proposed that, to a certain degree, nano-sized clay platelets carrying a negative charge serve as a dopant dopant
Any impurity added to a semiconductor to modify its electrical conductivity. The most common semiconductors, silicon and germanium, form crystalline lattices in which each atom shares electrons with four neighbours (see bonding). in the conducting polymer, and facilitate the delocalization of electrons, thus improving the conductivity. (9) The relationship between ionic and electrical properties with corrosion protection needs to be additionally investigated in future research projects.
Corrosion resistant properties of nanocomposites based on nonconductive polymer-layered silicates
There are also some references about the corrosion resistance of nanocomposite coatings based on layered silicates and conventional polymers like polysulfone (92) and other thermoplastic A polymer material that turns to liquid when heated and becomes solid when cooled. There are more than 40 types of thermoplastics, including acrylic, polypropylene, polycarbonate and polyethylene. polymers such as poly methylmethacrylate, (23) polystyrene, and thermosetting thermosetting,
adj having the property of becoming irreversibly rigid or hardened with the application of heat. In dentistry the term is used in connection with resins. polymers such as polyimide Pronounced "poly-ih-mid." A type of plastic (a synthetic polymeric resin) originally developed by DuPont that is very durable, easy to machine and can handle very high temperatures. Polyimide is also highly insulative and does not contaminate its surroundings (does not outgas). , (22), (93) epoxy, (94) and polyurethane. (95), (96)
Chen et al. (97) described the processing and different properties of epoxy layered-silicate nanocomposites as corrosion resistant coatings on Al (AA2024-T3) surfaces. They concluded that there is small improvement in the anticorrosion properties for the exfoliated nanocomposite coatings, and no improvement for the intercalated nanocomposites. It seems that these criteria are better related to the dispersion of silicate nanosheet in some epoxy matrix than the other grades of resin matrixes.
Some researchers have studied the corrosion resistance of polystyrene (PS)-clay and poly (styrene-co-acrylonitrile) (PSAN PSAN Partit Socialista d'Alliberament Nacional
PSAN Phase-Stabilized Ammonium Nitrate ) nanocomposites with quaternary alkyl alkyl /al·kyl/ (al´k'l) the monovalent radical formed when an aliphatic hydrocarbon loses one hydrogen atom.
n. ammonium salt as an intercalating agent. They concluded that these types of nanocomposite coatings on CRS were found to be a much superior anticorrosion over those of bulk PS and PSAN. Their conclusion was based on a series of electrochemical measurements of corrosion potential, polarization resistance, and corrosion current in 5 wt% aqueous NaCl electrolyte. Enhancement of anticorrosion properties of PS-claynanocomposites incorporated with low clay loading (e.g., 1 wt%) compared to bulk PS and PSAN might be comprised from dispersion of silicate nanolayers of clay in a polymer matrix. This enhancement is created by increasing the tortuosity tortuosity
1. The quality or condition of being tortuous; twistedness or crookedness.
2. A bent or twisted part, passage, or thing. of diffusion pathway for oxygen and water. (98), (99)
Yu et al. (22) have evaluated the anticorrosive properties of organo-soluble polyimide (TBAPP-PDA)/clay nanocomposite coatings derived from the solution dispersion technique. Based on a series of electrochemical measurements in aqueous NaCl electrolyte, they found that these soluble nanocomposite materials with low clay loading have much superior anticorrosion properties that those with soluble polyimide (SPI (1) (Stateful Packet Inspection) See stateful inspection.
(2) (Service Provider Interface) The programming interface for developing Windows drivers under WOSA. ) coatings. The effects of the material composition on barrier properties and optical clarity have also been studied. Gas permeability analyses show that the incorporation of clay platelets into an SPI membrane causes an enhancement of [0.sub.2] and [H.sub.2]O molecular barrier properties. Due to the better dispersion of nanoclay and more smooth surface morphology, the insoluble polyimide clay nanocomposite membranes have better barrier properties than the soluble polyimide clay nanocomposite membranes. Higher clay loading in SPI membranes leads to a significant decrease of optical clarity, as obtained from the UV-visible transmission spectra studies. (22)
Diffusion of moisture through vinyl ester Vinyl Ester, or Vinylester, is a resin produced by the esterification of an epoxy resin with an unsaturated monocarboxylic acid. The reaction product is then dissolved in a reactive solvent, such as styrene, to a 35 - 45 percent content by weight. nanocomposite coatings composed of MMT clay has been studied. It was found that water diffusivity Dif`fu`siv´i`ty
n. 1. Tendency to become diffused; tendency, as of heat, to become equalized by spreading through a conducting medium. is decreased by increasing clay content. Regardless of the nature of clay surface treatment, decreasing water diffusivity to half of its value in the neat resin will occur when the clay content is only 1 wt%. (100)
Siloxane-modified epoxy resin clay nanocomposite coatings with advanced anticorrosive properties have been prepared by a solution dispersion method. Better protection against corrosion on CRS coupons has been observed in comparison to that of bulk epoxy resin. Molecular permeability (e.g., [O.sub.2], [N.sub.2], and [H.sub.2]O), through epoxy resin-clay nanocomposite membranes, was lower than the bulk epoxy resin, along with the loading of nanoclay. These findings resulted from the gas and vapor permeability analysis. (101)
Yeh et al. (92) studied the corrosion prevention properties of polysulfone-clay (PSF-Clay) nanocomposite materials prepared by a solution dispersion method. They found that the prepared PCN coatings with low clay loading (1 wt%) on CRS were superior in corrosion prevention compared with bulk PSF using different chemical and electrochemical measurements in a 5 wt% aqueous NaCl electrolyte. (92)
The corrosion resistances of polyphenylenesulfide (PPS (Packets Per Second) The measurement of activity in a local area network (LAN). In LANs such as Ethernet, Token Ring and FDDI, as well as the Internet, data is broken up and transmitted in packets (frames), each with a source and destination address. )/MMT clay nanocomposite coatings have also been studied. It was found that MMt-PPS nanocomposite coating was effective in mitigating corrosion compared with MMT-free coating and, in fact, the uptake of corrosive ionic electrolyte by unmodified coating increased with an extended exposure time. (102)
Recently, the effects of using the organophilic MMT additives on the properties of epoxy coatings have been evaluated. It was concluded that the addition of organophilic layered silicates in epoxy systems results in improved coating properties such as adhesion, Persoz hardness, durability, gloss, water resistance, elasticity, and corrosion resistance. (103) In nonconductive polymeric nanocomposites, the addition of a small amount of suitable grade of clay increases the corrosion resistance and better protection of substrates in different conditions.
However, it seems that the research on the corrosion resistance of nonconductive PCN coatings is not complete and needs further efforts. Most of the previous work focused on the electrochemical and permeation properties without any attention to other specifications required for coatings, such as mechanical properties, adhesion, compatibility with other layers of coating systems, or type of surface pretreatment pretreatment,
n the protocols required before beginning therapy, usually of a diagnostic nature; before treatment.
n See predetermination. .
Recent studies on the use of conductive and nonconductive polymeric nanocomposites based on layered silicates have been reviewed. The use of clays within a composition of conductive polymer nanocomposites is a new area of research for obtaining coatings with tailored properties. The presence of the clay in nanoscale dispersion lengthens the diffusion path of corrosive media and improves barrier properties. Consequently, the lifetime of the conductive polymer coatings can be significantly improved by incorporation of the clay.
Thus, layered silicates play an important role in terms of providing barrier properties and high impedance In electronics, high impedance (also known as hi-Z, tri-stated, or floating) is the state of an output terminal which is not currently driven by the circuit. for the coating systems, which lead to improvement in corrosion protection. It is believed that, due to strong homogeneous impervious layers, the good corrosion protection properties of PCN coatings prevent corrosive media from seeping through it. As a result, clay-based nanocomposite coatings may be considered energy-saving and environment-friendly materials. The future of these special coating markets will further expand in different industries such as marine, building, construction, and defense. Finally, it must be considered that for industrial and commercial application of PCN coatings, they must be robust systems available in sufficient quantities at an acceptable price. It also must provide an equivalent or better performance in the field. The ancillary equipment used to apply the coatings must be also available. The challenge that still remains is a better understanding of the process and their reorganization of characteristics, and finding a protection mechanism for these materials. By solving these problems, an environmentally friendly coating material coating material,
n a biologically acceptable, usually porous nonmetal applied over the surface of a metallic implant with the expectation that tissue ingrowth will occur in the pores. Often a carbon polymer or ceramic substance. at a reasonable cost will be achieved.
(1.) Deberry, DW, "Modification of the Electrochemical and Corrosion Behavior of Stainless Steels with an Elcctroactive Coating." .J. Electrochem. Soc, 132 (5) 1022-1026 (1985)
(2.) Wessling, B, "On the Structure of Binary Conductive Polymer/Solvent Systems."' Synth. Met., 41 (!) 907-910 (1991)
(3.) Lu, WK, Elsenbaumer. RL. Wessling. B. "Corrosion Protection of Mild Steel by Coatings Containing Polyaniline." Synth. Met., 71 (1-3) 2163-2166 (1995)
(4.) Wrobleski, DA, Benicewicz, BC, Thompson, KG, Byrait, CJ "Corrosion Resistant Coatings From Conducting Polymers.1' Polym. Prepr. (Am. Chem. Soc, Div. Polym. Chem.). 35 (1) 265-266(1994)
(5.) Wessling, B, "Passivation passivation
the final stage in instrument manufacture, passing the finished instruments through a bath of nitric acid which removes foreign particles and promotes the formation of a protective coating of chromium oxide. of Metals by Coating with Poly-aniline: Corrosion Potential Shift and Morphological Changes." Adv. Mater., 6 (3) 226-228 (1994)
(6.) Yen, W, Jianguo. W. Xinri. J, Yeh, JM, Spellane, P, "Polyaniline as Corrosion Protection Coatings on Cold Rolled Steel."' Polymer, 36 (23) 4535-4537 (1995)
(7.) EPA Federal Register. "National Emission Standards for Hazardous Air Pollutants for Source Categories: Aerospace Manufacturing and Rework Facilities," 60 45947 (1995)
(8.) Skotheim, TA, Elsenbaumer. RL, Reynolds, JR, Handbook of Conducting Polymers. Marcel Dekker Marcel Dekker is a well-known encyclopedia publishing company with editorial boards found in New York, New York. They are part of the Taylor and Francis publishing group.
Initially a textbook publisher, they went to encyclopedia publishing in the late 1990's. (1998)
(9.) Zhu.Y. "Synthesis, Characterization and Corrosion Performance of Polyaniline-MontmoriNonile Clay Nanocomposites." PhD dissertation, College of Engineering Department of Chemical and Materials Engineering, Division of Research and Advanced Studies. University of Cincinnati The University of Cincinnati is a coeducational public research university in Cincinnati, Ohio. Ranked as one of America’s top 25 public research universities and in the top 50 of all American research universities, (2003)
(10.) Ramazan, A, Richard, OC, "Corrosion Protection of Materials by Applying Nanotechnology Associated Studies." Mat. Res. Soc. Symp. Proc. 788 L11. 44. 1 (2004)
(11.) Sanchez. C. Soler-illia. GJ de A A. Ribot. F, Lalot, T, Mayer, CR. Cabuil, V, "Designed Hybrid Organic-Inorganic Nano-composites from Functional Nanobuilding Blocks." Chem. Mater.. 13 (10) 3061-3083 (2001)
(12.) Ogawa. M, Kuroda, K, "Preparation of Inorganic-Organic Nanocomposites through Intercalation of Organoammonium Ions into Layered Silicates.'" Bull. Chem. Soc. Jpn., 70 (11) 2593-2618(1997)
(13.) Alexandre. M. Dubois. P, "Polymer Layered-Silicate Nanocomposites: Preparation, Properties and Use of a New Class of Materials." Mater. Sci. Eng R. Report. 28 (1-2) 1-63 (2000)
(14.) Ke, YC, Strove, P, Polymer Layered Silicate, Silica Nanocomposites. Elsevier. Amsterdam (2005)
(15.) Ruiz-Hilzky, E, ""Functionalizing Inorganic Solids: Towards Organic-Inorganic Nanostructured Materials for Intelligent and Bio-inspired Systems."' Chem. Rec, 3 (2) 88-100 (2003)
(16.) Ruiz-Hilzky, E, "Nanostructured. Functional Hybrid Materials." In: Gomez-Romero. P. Sanchez, C (eds.) Functional Hybrid Materials, p. 15. Wiley-VCH, Weinheim (2004)
(17.) Ruiz-Hilzky, E, Aranda, P, "Electroactive Polymers Intercalated in Clays and Related Solids." In: Pinnavaia, TJ, Beall, GW (eds.) Polymer-Clay Nanocomposites, pp. 18-46. John Wiley & Sons, New York New York, state, United States
New York, Middle Atlantic state of the United States. It is bordered by Vermont, Massachusetts, Connecticut, and the Atlantic Ocean (E), New Jersey and Pennsylvania (S), Lakes Erie and Ontario and the Canadian province of (2000)
(18.) Ruiz-Hilzky, E, Meerbeeck, AV. "Polymer-Clay Nanocomposites."' In: Bergaya. F, Theng, BKG BKG Background
BKG Bundesamt für Kartographieund Geodäsie (German: Federal Agency for Cartography and Geodesy)
BKG Background File . Lagaly, G (eds.) Handbook of Clay Science, pp. 583-623. Elsevier. Dordrecht (2006)
(19.) Aranda, P. Darder. M, Fcrnandez-Saavedra, R, Lopez-Blanco, M, Ruiz-Hilzky, E, "Relevance of Polymer and Biopolymer-Clay Nanocomposites in Electrochemical and Electroanalytical Applications." Thin Solid Films. 495 (1-2) 104-112(2006)
(20.) Yeh. JM. Liou, SJ, Lai, CY. Wu, PC. Tsai. TY. "Enhancement of Corrosion Protection Effect in Polyaniline via the Formation of Polyaniline - Gay Nanoeomposile Materials." Chem. Mater.. 13"(3) 1131-1136 (2001)
(21.) Yeh, JM, Chen. CL. Chen, YC Ma. CY. Lee, KR, Wei, Y, Li. S. "Enhancement of Corrosion Protection Effect of Poly (o-ethoxyaniline) via the Formation of Poly (o-elhoxyani-line)-Clay Nanocomposite Materials." Polymer, 43 (9) 2729-2736 (2002)
(22.) Yu, YH. Yeh. JM. Liou. SJ. Chang. YP, "Organo-Soluble Polyimide (TBAPP-OPDA)/Clay Nanocomposite Materials with Advanced Anticorrosive Properties Prepared from Solution Dispersion Technique." Acta Mater.. 52 (2) 475-486 (2004)
(23.) Yeh. JM. Liou, SJ. Lin. CY. Cheng. CY. Chang. YW, Lee. KR, "Anticorrosively Enhanced PMMA-clay Nanocomposite Materials with Qualemary Alkylphosphonium Salt as an Intercalating Agent." Chem. Mater.. 14 (1) 154-161 (2002)
(24.) Li. P. Tan. T'C. Lee, JY. "Corrosion Protection of Mild Steel by Electroactive Polyaniline Coatings." Synth. Met., 88 (3) 237-242(1997)
(25.) Zeng, OH, Yu, AB, Lu, GQ(Max). Paul, DR. "Clay-Based Polymer Nanocomposites: Research and Commercial Development." .J. Nanosci Nanoteclmol.S (1) 1574-1592 (2005)
(26.) Krishnamoorti. R, Vaia, RA, Polymer Nanocomposites: Synthesis, Characterization and Modeling. American Chemical Society The American Chemical Society (ACS) is a learned society (professional association) based in the United States that supports scientific inquiry in the field of chemistry. Founded in 1876 at New York University, the ACS currently has over 160,000 members at all degree-levels and in . Washington DC (2001)
(27.) Komarneni. SK, "Nanophase and Nanocomposite Materials." IV: Materials Research Society Symposium Proceedings Symposium, Boston, Massachusetts. October 2001
(28.) Giannelis, EP, "Polymer Layered Silicate Nanocomposites." Adv. Mater., 8 (1) 29-35 (1996)
(29.). Lagaly, G. "From Clay Mineral-Polymer Interactions to Clay Mineral-Polymer Nanocomposites." Appl. Clay Sci, 15 (1-2) 1-9(1999)
(30.) Lebaron, PC, Wang, Z, Pinnavaia. TJ, "Polymer-layered Silicate Nanocomposites: An Overview." Appl. Clav Sci.. 15 (1-2) 11-29(1999)
(31.) Oriakhi. CO, "Microstruclure of the Inorganic Polymer Nanocomposition Approach to Advanced Materials." .J. Chem. Educ. 11 (9) 1138-1146 (2000)
(32.) Schmidt, D. Shah, D. Giannelis, EP, "'New Advances in Polymer/Lave red Silicate Nanocomposites." Cttrr Opin Solid Slate Mater Sci, 6 (1) 205-212 (2002)
(33.) Biswas, M, Ray, S, "Recent Progress in Synthesis and Evaluation of Polymer Montmorillonite Nanocomposites." Adv. Polvm. Sci. 155 (I) 167-221 (2001}
(34.) Ray, S, Okamoto, M, "Polymer/Layered Silicate Nanocomposites: A Review from Preparation to Processing." Prog. Polym. Sci.. 28 (11) 1539-1641 (2003)
(35.) Kawasumi. M. "The Discovery of Polymer-Clay Hybrids." .J. Polym. Sci. Part A: Polym. Chem.. 42 (4) 819-824 (2004)
(36.) Yoshimoto, S, Ohashi, F, Ohnishi, Y, Nonamib, T, "Synthesis of Polyaniline-Montmorillonite Nanocomposites by the Mechanochemical mech·a·no·chem·i·cal
Of or relating to conversion of chemical energy into mechanical work. Intercalation Method." Svnth. Met.. 145 (2-3) 265-270 (2004)
(37.) JJicng, BKG, The Chemistry of Clay-Organic Reactions. John Wiley & Sons, New York (1974)"
(38.) Ben-Hur, M, Malik, M, Letey. J, Mingelgrin, U. "Adsorption adsorption, adhesion of the molecules of liquids, gases, and dissolved substances to the surfaces of solids, as opposed to absorption, in which the molecules actually enter the absorbing medium (see adhesion and cohesion). of Polymers on Clays as Affected bv Clay Charge and Structure. Polymer Properties and Water." Soil Sci.. 153 (5) 349-356(1992)
(39.) Hirsch. D. Nir. S. Banin. A. "Prediction of Cadmium Complexation in Solution and Adsorption to Montmorillonite." Soil Sci Soc Am. J., 53 (3) 716-721 (1989)
(40.) Zhang, Z, Sparks, DL. Scrivner. NC, "Sorption sorption /sorp·tion/ (sorp´shun) the process or state of being sorbed; absorption or adsorption.
Adsorption or absorption. and Desorption Desorption
A process in which atomic and molecular species residing on the surface of a solid leave the surface and enter the surrounding gas or vacuum. of Quaternary Amine amine (əmēn`, ăm`ēn): see under amino group.
Any of a class of nitrogen-containing organic compounds derived, either in principle or in practice, from ammonia (NH3). Cations on Clays." Environ. Sci. Technol., 27 (8) 1625-1631 (1993)
(41.) Kaviratna, PD. Pinnavaia, TJ, Schroeder, PA, "Dielectric Properties of Smectite Clays." J Phys. Chem. Solids, 57 (12) 1897-1906(1996)
(42.) Karaborni. S, Smit, B. Heidug. W. Urai. J, Van Oort, F, "The Swelling of Clays: Molecular Simulations of the Hydration hydration /hy·dra·tion/ (hi-dra´shun) the absorption of or combination with water.
1. The addition of water to a chemical molecule without hydrolysis.
2. of Montmorillonite," Science, 271 (5252) 1102-1104(1996)
(43.) Blumslein, A, "Polymerization of Adsorbed Monolayers: IT. Thermal Degradation of the Inserted Polymers." J. Polym. Sci., 3 (7)2665-2673 (1965)
(44.) Krishnamoorti. R, Vaia, RA, Giannelis, EP, "Structure and Dynamics of Polymer Layered Silicate Nanoeomposites." Chem. Mater.. 8 (8) 1728-1734 (1996)
(45.) Sung, JH. Choi, HJ, "Electrorheological Characteristics of Poly (o-ethoxy) aniline aniline (ăn`əlĭn), C6H5NH2, colorless, oily, basic liquid organic compound; chemically, a primary aromatic amine whose molecule is formed by replacing one hydrogen atom of a benzene molecule with an amino Nanocomposite." Kor kor
[Hebrew kôr, from Akkadian kurru, from Sumerian gur, a unit of measurement.]
Noun 1. .-Aust. Rheol. .J., 16 (4) 193-199(2004)
(46.) Vadivel. A. Synthesis- and Characterization of Organo-Inorganic Conductive Polymer Based Nanocomposites for Electrochemical Power Sources. University of Pune History
The University of Pune was established under the Poona University Act, passed by the Bombay legislature on February 10, 1948. In the same year, Dr. M.R. Jayakar assumed office as the first vice chancellor of the university. Shri B.G. , Pune (2004)
(47.) Okada, A, Kawasumi, M. Usuki. A, Kojima. Y, Kurauchi, T, Kamigaito, O, "Synthesis and Properties of Nylon-6/Clay Hybrids." In: Schaefer. DW, Mark. JE (eds.) Polymer Based Molecular Composites, pp. 45-50. MRS MRS - Modifiable Representation System.
An integration of logic programming into Lisp.
["A Modifiable Representation System", M. Genesereth et al, HPP 80-22, CS Dept Stanford U 1980]. Symposium Proceedings, Pittsburgh (1990)
(48.) Giannelis, EP. Krishnamoorti. R, Manias, E, "Polymer-Silicate Nanocomposites: Novel Systems for Confined Polymers and Polymer Brushes." Adv. Polym. Sci, 138 (I) 107-147 (1999)
(49.) Vaia, RA. Price, G. Ruth, PN, Nguyen, I IT, Lichlen. J, "Polymer/Layered Silicate Nanocomposites at High Performance Ablative ablative (ăb`lətĭv') [Lat.,=carrying off], in Latin grammar, the case used in a number of circumstances, particularly with certain prepositions and in locating place or time. The term is also used in the grammar of some languages (e.g. Materials." Appl Clay Sci. .15(1) 67-92 (1999)
(50.) Kryszewski, M, "Nanointercalates-Novei Class of Materials with Promising Properties."' Synth. Mel., 109 (1) 47-54 (2000)
(51.) Ray. S, Okamoto, M, Okamoto, K, "Structure-Property Relationship in Biodegradable Poly (butylenes Succinate succinate /suc·ci·nate/ (suk´si-nat) any salt or ester of succinic acid.
succinate semialdehyde ?.
n. )/ Layered Silicate Nanocomposites." Macromolecules Macromolecules
A large molecule composed of thousands of atoms.
Mentioned in: Gene Therapy
macromolecules , 36 (7) 2355-2367 (2003)
(52.) Walls, HJ. Riley. MW. Singhal. RR, Sponlak. RJ, Fedkiw, PS. Khan, SA. "Nanocomposite Electrolytes with Fumed fume
1. Vapor, gas, or smoke, especially if irritating, harmful, or strong.
2. A strong or acrid odor.
3. A state of resentment or vexation.
v. Silica and Hectorite Clay Networks: Passive versus Active Fillers.'" Adv. Fund. Mater.. 13 (9) 710-717 (2003)
(53.) Usuki, A, Kojima, Y, Kawasumi, M, Okada, A, Fukushima, Y, Kurauchi. T, Kamigaito, O, "Synthesis of Nylon 6-Clay Hybrid."./. Mater. Res.,8(5) 1179-1184(1993) '
(54.) Decker, C, Keller, L, Zahouily, K, Benfarhil, S. "Synthesis of Nanocomposite Polymers by UV-Radiation Curing." Polymer, 46 (17) 6640-6648 (2005)
(55.) Oilman Oil´man
n. 1. One who deals in oils; formerly, one who dealt in oils and pickles.
2. A person working in the petroleum industry, esp. an oil company executive.
Noun 1. , JW, "Flammability and Thermal Stability Studies of Polymer Layered-Silicate Clay Nanocomposites." Appi. Clay Sci., 15 (1-2) 31-49 (1999)
(56.) Ogasawara, T, lshida, Y, Ishikawa, T. Aoki, T, Ogura, T, "Helium Gas Permeability of Montmorillonite/Epoxy Nanocomposites." Composites: Pan A. 37 (12) 2236-2240 (2006)
(57.) Oilman, JW, Kashiwagi, T, Morgan, AB. Harris, RH. Brassell, L, VanLandingham, M, Jackson, (X, "Flammability of Polymer Clay Nanocomposite Consider: Year One Report."" NIST (National Institute of Standards & Technology, Washington, DC, www.nist.gov) The standards-defining agency of the U.S. government, formerly the National Bureau of Standards. It is one of three agencies that fall under the Technology Administration (www.technology. 1R 6531. July 2000
(58.) Kim. BH. Jung, JH. Joo. J. Epstein. AJ, Mizoguchi. K. Kim, JW. Choi, HJ. "Nanocomposite of Polyaniline and Na + Montmorillonite Clay." Macromolecules, 35 (4) 1419-1423 (2002)
(59.) Kornmann, X, Lindbergh. H, Berglund, LA, "Synthesis of Epoxy-Clay Nanocomposites: Influence of the Nature of the Clay on Structure."" Polymer, 42 (4) 1303-1310 (2001)
(60.) Agag, T, Koga. T. Takeichi, T, "Studies on Thermal and Mechanical Properties of Polyimide-Clay Nanocomposites." Polymer. 42 (8) 3399-3408 (2001)
(61.) Wessling. B, "Dispersion as the Link Between Basic Research and Commercial Applications of Conductive Polymers (Polyaniline)." Synth. Met.. 93 (2) 143-154 (1998)
(62.) Wessling, B, "From Conductive Polymers to Organic Metals."' Am. Chem. Sac. 31 (1) 34-40 (2001)
(63.) Stenger-Smilh, J, "A General Review of Intrinsically Conducting Polymers as Coatings for Corrosion Protection." Proc. U.S. Navy & Industry Corrosion Technology Information Exchange, Louisville. KY, July 2000
(64.) Sitaram, S. Stoffer, J, O'Keefe, T, "Application of Conducting Polymers in Corrosion Protection." J. Coat. Technol. (USA), 69 (866) 65-69 (1997)
(65.) Wessling, B, Posdorfe, .J, "Corrosion Prevention with an Organic Metal (polyaniline): Corrosion Test Results." Electrochim. Acta. 44 (12) 2139-2147 (1999)
(66.) Samui, AB, Patankar, AS, Rangarajan, J, Deb. PC. "Study of Polyaniline Containing Paint for Corrosion Prevention." Prog. Org. Coat., 47 (1) 1-7 (2003)
(67.) Twite twite
A small songbird (Carduelis flavirostris) of northern Great Britain and Scandinavia that resembles the linnet.
[Imitative of its call.] , RL. Bierwagen, GP, "Review of Alternatives to Chromate for Corrosion Protection of Aluminum Aerospace Alloys." Prog. Org. Coat.. 33 (2) 91-100 (1998)
(68.) Kinlen, P.I. Silverman, DC, Jeffreys. CR, "Corrosion Protection Using Polyaniline Coating Formulations.(1) Synth. Met., 85 (1) 1327-1332 (1997)
(69.) Wessling. B. Schroder, S, Gleeson, S, Merkle, H, Schroder, S. Baron, F, "Reaction Scheme for the Passivation of Metals by Polyaniline." Mater. Corros., 47 (87) 439-445 (1996)
(70.) Liu, LM. Levon, K, "Undoped Polyaniline-Surfactant Complex for Corrosion Prevention." .J. Appl Polym. Sci,, 73 (14) 2849-2856 (1999)
(71.) Bacskai, R. Schroeder, AH, Young, DC, "Hydrocarbon-Soluble Alkaline/Formalin/Formaldehyde Oligomers as Corrosion Inhibitors." ,J, Appl Polym. Sci, 42 (9) 2435-2441 (1991)
(72.) Kinlen, PJ, Menon, V, Ding, Y, "A Mechanistic Investigation of Polyaniline Corrosion Protection Using the Scanning Reference Electrode Technique." .J. Electrochem. Soc, 146 (10) 3690-3695 (1999)
(73.) Shah, K, Iroh. J, "Electrochemical Synthesis and Corrosion Behavior of Poly (N-ethyl aniline) Coatings on Al-2024 Alloy."" Synth Met.. 132 (1) 35-41 (2002)
(74.) Spellane. P. Yahkind. A. Abu-shanab. O. "Metal Corrosion Protection with Wash Coat of Polyphenylene Oxide." US Patent 6.004.628, 1999
(75.) Feser. R, Erning, W, "Corrosion Inhibition of Magnesium under Organic Coatings by Self Assembling Molecules." Paper Presented at European Coating Conference, Proceedings European Coatings Conference, Anticorrosive Pigments, Berlin. June 2000
(76.) Epstein, AJ. Jasty. SG, "Corrosion Protection of Iron/Steel by Emeraldine Base Polyaniline.'" United States Patent 5972518, October 1999
(77.) Schauer. T, Joos, A, Duo, L, Eisenbach, CD, "Protection of Iron Against Corrosion with Polyaniline Primers." Prog. Org. Coal.. 33 (1) 20-27 (1998)
(78.) Qiang. M. Chen. T, Yao, RP. Chen. L. "Effect of Preparation Condition of Polyaniline-Monmorillonile Nanocompos-ite Material on the Anticorrosion Property."' Mater. Protect. (China), 36 (7) 25-27 (2003)
(79.) Yeh, JM, Chin, CP. "Structure and Properties of Poly (o-methoxyaniline)-Clay Nanocomposite Materials." J. Appl Polym. Sci., 88 (4) 1072-1080 (2003)
(80.) Yu, YH, Jen, CC, Huang. HY, Wu, PC, Huang. CC, Yeh. JM, ''Preparation and Properties of Heterocyclically Conjugated conjugated
estrogens, conjugated Warning - Hazardous drug!
C.E.S. Poly (3-hexylthiophene)-Clay Nanocomposite." .J. Appl Polym. Sci 91 (6) 3438-3446 (2004)
(81.) Yeh, JM, Chin, CP, Chang, S, -'Enhanced Corrosion Protection Coatings Prepared from Soluble Electronically Conductive Polypyrrole-Clay Nanocomposite Materials." .J. Appl Polym. Sci, 88 (14) 3264-3272 (2003)
(82.) Ding, K, Jia, Z, Ma, W, Tong, R, Wang. X. "Polyaniline and Polyaniline-Thiokol Rubber Composite Coatings for the Corrosion Protection of Mild Steel." Mater. Chem. Phys.. 76 (2) 137-142 (2002)
(83.) Tan, CK, Blackwood, DJ, "Corrosion Protection by Multi Layered Conducting Polymer Coatings." Corros. Sci, 45 (3) 545-557 (2003)
(84.) lvanov, S, Mokreva. P. Tsakova, V. Terlemezyan, L, "Electrochemical and Surface Structural Characterization of Chemically and Electrochemically Synthesized Polyaniline Coatings." Thin Solid films. 441 (1-2) 44-49 (2003)
(85.) Beck, F, Michaelis, R, Schloten, F. Zinger zing·er
1. A witty, often caustic remark.
2. A sudden shock, revelation, or turn of events.
Noun 1. , B, "Filmforming Electropolymerization of Pyrrole on Iron in Aqueous Oxalic-Acid." Electrochim, Acta, 39 (2) 229-234 (1994)
(86.) Rajagopalan. R, Iroh. JO, "Development of Polyaniline-Polypyrrole Composite Coatings on Steel by Aqueous Electrochemical Process." Electrochim. Acta, 46 (16) 2443-2455 (2001)
(87.) Su.W.Iroh.JD, "Electrodeposition e·lec·tro·de·pos·it
tr.v. e·lec·tro·de·pos·it·ed, e·lec·tro·de·pos·it·ing, e·lec·tro·de·pos·its
To deposit (a dissolved or suspended substance) on an electrode by electrolysis.
The substance so deposited. Mechanism. Adhesion and Corrosion Performance of Polypyrrole and Poly (N-methyl-pyrrole) Coatings on Steel Substrates." Synth. Met., 114 (3) 225-234 (2000)
(88.) Yeh. JM. Chin, CP. Chang. S. "Enhanced Corrosion Protection Coatings Prepared From Soluble Electronically Conductive Polypyrrole-Clay Nanocomposite Materials." J. Appl. Polym. Sci, 88 (14) 3264-3272 (2003)
(89.) Mravakova. M. Boukerma, K. Omastova, M. Chehimi. MM. "Monlmorillonite/Polypyrrole Nanocomposites the Effect of Organic Modification of Clay on the Chemical and Electrical Properties." Mater. Sci Eng.. 26 (2-3) 306-313 (2006)
(90.) Chang. KC Lai, MC. Peng. CW. Chen. YT, Yeh. JM. Lin. CL, Yang, JC, "Comparative Studies on the Corrosion Protection Effect of DBSA-Doped Polyaniline Prepared From In Situ Emulsion Polymerization in the Presence of Hydrophilic Na+-MMT and Organophilie Organo-MMT Clay Platelets." Electrochim. Acta". 51 (26) 5645-5653 (2006)
(91.) Mehrota, V. Giannelis, EP, "Metal-Insulator Molecular Multilayers of Electroactive polymers: Intercalation of Polyaniline in Mica-type Layered Silicates." Solid State Commun., 77 (2) 155-158 (1991}
(92.) Yeh, JM. Chen, CL. Chen. YC, Ma, CY, Huang, HY, Yu. YH. "Enhanced Corrosion Prevention Effect of Polysulfone-Clay Nanocomposite Materials Prepared by Solution Dispersion." .J. Appl Polym. Sci, 92 (1) 631-637 (2004)
(93.) Yeh, JM. Hsieh. CF. Jaw, JH. Kuo, TH, Huang. HY, Lin, CL. Hsu. MY. "Organo-soluble Polyimide (ODA-BSAA)/ Montmorillonite Nanocomposite Materials Prepared by Solution Dispersion Technique." J. Appl Polym. Sci, 95 (5) 1082-1090 (2005)
(94.) Becker. O. Varley, RJ, Simon. GP. "Thermal Stability and Water Uptake of High Performance Epoxy Layered Silicate Nanocomposites." Eur. Polym. .J., 40 (1) 187-195 (2004)
(95.) Solarski, S, Benali, S, Rochery, M. Devaux, E, Alexandre, M. Monteverde, F. Dubois, P. "Synthesis of a Polyurethane/ Clay Nanocomposite Used as Coating: Interactions between the Counterions of Clay and the Isocyanate i·so·cy·a·nate
Any of a family of nitrogenous chemicals that are used in industry and can cause respiratory disorders, especially asthma, if inhaled. and Incidence on the Nanocomposite Structure." .J. Appl. Polym. Sci, 95 (2) 238-244 (2004)
(96.) Ma, J, Zhang, S, Qi. Z. "Synthesis and Characterization of Elastomeric Polyurethane/Clay Nanocomposites." .L. Appl Polym. Sci., 82 (6) 1444-1448 (2001)
(97.) Chen. C. Khobaib. M, Curliss. D. "Epoxy Layered-Silicate Nanocomposites." Prog. Org. Coat., 47 (3-4) 376-383 (2003)
(98.) Yeh. JM, Liou, S.I, Lin, CG, Chang, YP, Yu, YH, Cheng, CF, "Effective Enhancement of Anticorrosive Properties of Polystyrene by Polystyrene-Clav Nanocomposite Materials." .J. Appl Polym. Sci. 92 (3) 1970-1976 (2004)
(99.) Yeh, JM, Liou, SJ. Lu, HJ, Huang, HY, "Enhancement of Corrosion Protection Effect of Poly(styrene-co-acrylonitrile) by the Incorporation of Nanolayers of Montmorillonite Clay into Copolymer copolymer: see polymer. Matrix." .J. Appl Polym. Sci. 92 (4) 2269-2277 (2004)
(100.) Shah, AP, Gupta, RK, Gangarao, HVS HVS Human Visual System
HVS Herpesvirus Saimiri
HVS High Voltage Software
HVS High-Volume Sampler
HVS Hard, Very Severe (rock climbing grade)
HVS Hue, Value, Saturation (color model, aka HLS) . Powell. CE, "Moisture Diffusion through Vinyl Ester Nanocomposites Made with Montmorillonite Clay." Polym. Eng. Sci, 42 (9) 1852-1863 (2004)
(101.) Yeh, JM, Huanga, HY. Chen. CL. Sua, WF, Yu. YH. "Siloxane-Modified Epoxy Resin-Clay Nanocomposite Coatings with Advanced Anticorrosive Properties Prepared by a Solution Dispersion Approach." Surf. Coat. Techno!., 200 (8) 2753-2763 (2006)
(102.) Sugama. T, "Polyphenylenesulfide/Montomorillonite Clay Nanocomposite Coatings: Their Efficacy in Protecting Steel against Corrosion." Mater. Lett, 60 (21-22) 2700-2706 (2006)
(103.) Garea, SA, lovu. H, "New Epoxy Coaling Systems Which Contain Multipurpose mul·ti·pur·pose
Designed or used for several purposes: a multipurpose room; multipurpose software.
Adjective Additives Based on Organophilic Montmorillonite." Prog. Org. Coat, 56 (4) 319-326 (2006)
D.Zaarei, A. A. Sarabi , F. Sharif, S.M.Kassiriha Polymer Faculty, Amirkabir University of Technology Amirkabir University of Technology (AUT, دانشگاه صنعتی امیرکبیر), formerly named Tehran Polytechnic , Tehran, Iran